Presentation on theme: "Lecture No. 8 Tests on Aggregates (cont.) Prepared by: Dr. Salah Al-Dulaijan."— Presentation transcript:
Lecture No. 8 Tests on Aggregates (cont.) Prepared by: Dr. Salah Al-Dulaijan
Bulck Density (ASTM C 29) Defined as the weight of the aggregate particles that would fill a unit volume. The term bulk is used since the volume is occupied by both the aggregates and voids. The typical bulk density used in making normal concrete ranges from 1200 to 1750 kg/m 3. The void contents range between 30% to 45% for coarse aggregate and 40% to 50% for fine aggregate. Void content increases with angularity and decreases with well graded aggregate.
Relative Density (Specific Gravity) The relative density of an aggregate (ASTM C 127 and C 128) is defined is the ratio of its mass to the mass of an equal absolute of water. It is used in certain computations for mixture proportioning and control. Most natural aggregates have relative densities between 2.4 and 2.9 (2400 and 2900 kg/ m 3 ). The density of aggregate used in mixture proportioning computations (not including the voids between particles) is determined by multiplying the relative density of the aggregate times the density of water (1000 kg/m 3 ).
Absorption and Surface Moisture The absorption and surface moisture of aggregates should be determined using ASTM C 70, C127, C128, and C 566 so that the total water content of the concrete can be controlled and the batch weights determined. The moisture conditions of aggregates are: Oven dray Air dry Saturated surface dry (SSD) Damp or wet
Absorption levels AggregateMoisture content at SSD (%) Free-water content (%) Coarse Fine
Moisture conditions of aggregate
Wetting and Drying Alternate wetting and drying can develop sever strain in some aggregates, and with certain types of aggregate this can cause a permanent increase in volume of concrete and eventual breakdown. Clay lumps and other friable particles can degrade when subjected to wetting and drying cycles. Also, moisture swelling of clay and shales can cause popouts in concrete.
Abrasion and Skid Resistance (ASTM C 131) Abrasion resistance of an aggregate is used as a general index of its quality. This characteristic is important when concrete is going to be subjected to abrasion, as in heavy duty floors or pavements. Low abrasion resistance may increase the quantity of fines in the concrete during mixing; and hence increases the water requirement and require an adjustment in w/c ratio. Los Angeles abrasion test as per ASTM C 131 is the most common test for abrasion test.
Strength Generally, strength of aggregate does not influence the strength of conventional concrete as much as the strength of the paste and the paste-aggregate strength. However, aggregate strength becomes important in high strength concrete. Aggregate tensile strengths range between 2 to 15 MPa, and compressive strengths range between 65 to 270 MPa.
Shrinkage Usually aggregates with high absorption may have high shrinkage on drying. Low shrinkage aggregatesHigh shrinkage aggregates Quartz, feldspar, limestone, dolomite, granite Sandstone, shale, slate, hornblende
Effect of type of aggregate on shrinkage
Resistance to Acid and other Corrosive Substances Acid solutions (pH less than 6.0) attack the calcium compounds of the cement paste, the rate of attack depends on the acidity of the solution. Siliceous aggregates may not be attacked by acidic solutions, however, calcareous aggregates often reacts with acids resulting in reduction of the solution acidity. Other gases and salts may attack and disintegrate concrete. Therefore, concrete structures subjected to harsh conditions should be protected and aggressive agents should be prevented from coming into contact with the concrete by using protective coatings.
Fire Resistance and Thermal Properties The fire resistance and thermal properties of concrete depend on the mineral constituents of the aggregates. Lightweight aggregates are more fire resistance than normal weight aggregates due to their insulation properties. Concrete containing calcareous coarse aggregates performs better under fire exposure than siliceous aggregate (granite or quartz).
Potentially Harmful Materials Aggregates are potentially harmful if they contain compounds known to react chemically with Portland cement and produce: –Volume change of the paste, aggregates, or both. –Affect the normal hydration of cement. –Harmful byproducts. Harmful materials present in aggregates are listed in Table 5-6: